#------------------------------------------------------------------------------
#$Date: 2016-03-21 17:50:02 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178794 $
#$URL: svn://www.crystallography.net/cod/cif/4/10/48/4104808.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4104808
loop_
_publ_author_name
'Peter D. Southon'
'Lang Liu'
'Elizabeth A. Fellows'
'David J. Price'
'Gregory J. Halder'
'Karena W. Chapman'
'Boujemaa Moubaraki'
'Keith S. Murray'
'Jean-François Létard'
'Cameron J. Kepert'
_publ_contact_author_address
; 
School of Chemistry
University of Sydney
NSW 2006
Australia
;
_publ_contact_author_email       c.kepert@chem.usyd.edu.au
_publ_contact_author_fax         +61-2-9351-3329
_publ_contact_author_name        'Prof. Cameron J. Kepert'
_publ_contact_author_phone       +61-2-9351-5741
_publ_section_title
;
 Dynamic Interplay between Spin-Crossover and Host-Guest Function in a
 Nanoporous Metal-Organic Framework Material
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              10998
_journal_page_last               11009
_journal_paper_doi               10.1021/ja902187d
_journal_volume                  131
_journal_year                    2009
_chemical_formula_moiety         'C8 H8 Fe N6 Ni O2'
_chemical_formula_sum            'C8 H8 Fe N6 Ni O2'
_chemical_formula_weight         334.76
_chemical_name_common            '[Fe(pz)Ni(CN)4].2H2O'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           47
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2 2'
_symmetry_space_group_name_H-M   'P m m m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   7.1139(3)
_cell_length_b                   6.9109(4)
_cell_length_c                   6.7799(3)
_cell_measurement_reflns_used    1415
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      29.922
_cell_measurement_theta_min      2.8635
_cell_volume                     333.32(3)
_computing_cell_refinement       'SAINT Ver. 7.23A  (Bruker-AXS, 2005)'
_computing_data_collection       'APEX2 Ver. 2.1-3 (Bruker-AXS, 2007)'
_computing_data_reduction        'SAINT Ver. 7.23A'
_computing_molecular_graphics    'XPMA/ZORTEP, WebLab Viewer 3.7'
_computing_publication_material  CIFTAB
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      150(2)
_diffrn_measured_fraction_theta_full 0.961
_diffrn_measured_fraction_theta_max 0.973
_diffrn_measurement_device_type  'Bruker-Nonius FR591 Kappa APEX II'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus rotating anode'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0117
_diffrn_reflns_av_sigmaI/netI    0.0118
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       3
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            2462
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         29.92
_diffrn_reflns_theta_min         2.86
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.502
_exptl_absorpt_correction_T_max  0.942
_exptl_absorpt_correction_T_min  0.837
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker-AXS, 2004)'
_exptl_crystal_colour            red-yellow
_exptl_crystal_density_diffrn    1.668
_exptl_crystal_description       'rectangular block'
_exptl_crystal_F_000             168
_exptl_crystal_size_max          0.071
_exptl_crystal_size_mid          0.024
_exptl_crystal_size_min          0.024
_refine_diff_density_max         1.039
_refine_diff_density_min         -0.550
_refine_diff_density_rms         0.162
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.118
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     38
_refine_ls_number_reflns         585
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.117
_refine_ls_R_factor_all          0.0394
_refine_ls_R_factor_gt           0.0334
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0446P)²+0.6984P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0885
_refine_ls_wR_factor_ref         0.0936
_reflns_number_gt                507
_reflns_number_total             586
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja902187d_si_001_2.cif
_cod_data_source_block           1.2H2O(150)
_cod_database_code               4104808
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'x, -y, -z'
'-x, y, -z'
'-x, -y, -z'
'x, y, -z'
'-x, y, z'
'x, -y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ni1 Ni 0.5000 0.5000 0.0000 0.0097(2) Uani 1 8 d S
Fe1 Fe 0.0000 0.0000 0.0000 0.0086(2) Uani 1 8 d S
O10 O 0.5000 0.203(2) 0.5000 0.059(3) Uiso 0.385(4) 4 d SP
O11 O 0.5000 0.0000 0.417(4) 0.059(3) Uiso 0.215(10) 4 d SP
O12 O 0.5000 0.413(5) 0.5000 0.059(3) Uiso 0.171(11) 4 d SP
O13 O 0.344(4) 0.5000 0.5000 0.059(3) Uiso 0.228(10) 4 d SP
N1 N 0.1948(3) 0.1973(4) 0.0000 0.0125(5) Uani 1 2 d S
N2 N 0.0000 0.0000 0.2929(5) 0.0122(6) Uani 1 4 d S
C1 C 0.3125(4) 0.3111(4) 0.0000 0.0125(5) Uani 1 2 d S
C2 C 0.0000 0.1641(5) 0.3972(4) 0.0178(6) Uani 1 2 d S
H2 H 0.0000 0.2843 0.3292 0.021 Uiso 1 2 calc SR
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
C1 Ni1 C1 180.0 5_665 .
C1 Ni1 C1 91.25(17) 5_665 3_565
C1 Ni1 C1 88.75(17) . 3_565
C1 Ni1 C1 88.75(17) 5_665 7_655
C1 Ni1 C1 91.25(17) . 7_655
C1 Ni1 C1 180.0 3_565 7_655
C1 Ni1 O12 83.0(4) 5_665 5_666
C1 Ni1 O12 97.0(4) . 5_666
C1 Ni1 O12 83.0(4) 3_565 5_666
C1 Ni1 O12 97.0(4) 7_655 5_666
C1 Ni1 O12 97.0(4) 5_665 1_554
C1 Ni1 O12 83.0(4) . 1_554
C1 Ni1 O12 97.0(4) 3_565 1_554
C1 Ni1 O12 83.0(4) 7_655 1_554
O12 Ni1 O12 180.000(1) 5_666 1_554
C1 Ni1 O12 97.0(4) 5_665 .
C1 Ni1 O12 83.0(4) . .
C1 Ni1 O12 97.0(4) 3_565 .
C1 Ni1 O12 83.0(4) 7_655 .
O12 Ni1 O12 20.1(11) 5_666 .
O12 Ni1 O12 159.9(11) 1_554 .
C1 Ni1 O12 83.0(4) 5_665 5_665
C1 Ni1 O12 97.0(4) . 5_665
C1 Ni1 O12 83.0(4) 3_565 5_665
C1 Ni1 O12 97.0(4) 7_655 5_665
O12 Ni1 O12 159.9(11) 5_666 5_665
O12 Ni1 O12 20.1(11) 1_554 5_665
O12 Ni1 O12 180.0(11) . 5_665
C1 Ni1 O13 77.2(3) 5_665 5_666
C1 Ni1 O13 102.8(3) . 5_666
C1 Ni1 O13 102.8(3) 3_565 5_666
C1 Ni1 O13 77.2(3) 7_655 5_666
O12 Ni1 O13 20.6(4) 5_666 5_666
O12 Ni1 O13 159.4(4) 1_554 5_666
O12 Ni1 O13 20.6(4) . 5_666
O12 Ni1 O13 159.4(4) 5_665 5_666
C1 Ni1 O13 102.8(3) 5_665 1_554
C1 Ni1 O13 77.2(3) . 1_554
C1 Ni1 O13 77.2(3) 3_565 1_554
C1 Ni1 O13 102.8(3) 7_655 1_554
O12 Ni1 O13 159.4(4) 5_666 1_554
O12 Ni1 O13 20.6(4) 1_554 1_554
O12 Ni1 O13 159.4(4) . 1_554
O12 Ni1 O13 20.6(4) 5_665 1_554
O13 Ni1 O13 180.0 5_666 1_554
C1 Ni1 O13 102.8(3) 5_665 .
C1 Ni1 O13 77.2(3) . .
C1 Ni1 O13 77.2(3) 3_565 .
C1 Ni1 O13 102.8(3) 7_655 .
O12 Ni1 O13 20.6(4) 5_666 .
O12 Ni1 O13 159.4(4) 1_554 .
O12 Ni1 O13 20.6(4) . .
O12 Ni1 O13 159.4(4) 5_665 .
O13 Ni1 O13 36.2(8) 5_666 .
O13 Ni1 O13 143.8(8) 1_554 .
C1 Ni1 O13 77.2(3) 5_665 5_665
C1 Ni1 O13 102.8(3) . 5_665
C1 Ni1 O13 102.8(3) 3_565 5_665
C1 Ni1 O13 77.2(3) 7_655 5_665
O12 Ni1 O13 159.4(4) 5_666 5_665
O12 Ni1 O13 20.6(4) 1_554 5_665
O12 Ni1 O13 159.4(4) . 5_665
O12 Ni1 O13 20.6(4) 5_665 5_665
O13 Ni1 O13 143.8(8) 5_666 5_665
O13 Ni1 O13 36.2(8) 1_554 5_665
O13 Ni1 O13 180.0 . 5_665
N1 Fe1 N1 180.00(15) . 5
N1 Fe1 N1 89.09(14) . 3
N1 Fe1 N1 90.91(14) 5 3
N1 Fe1 N1 90.91(14) . 7
N1 Fe1 N1 89.09(14) 5 7
N1 Fe1 N1 180.00(10) 3 7
N1 Fe1 N2 90.0 . 5
N1 Fe1 N2 90.0 5 5
N1 Fe1 N2 90.0 3 5
N1 Fe1 N2 90.0 7 5
N1 Fe1 N2 90.0 . .
N1 Fe1 N2 90.0 5 .
N1 Fe1 N2 90.0 3 .
N1 Fe1 N2 90.0 7 .
N2 Fe1 N2 180.0 5 .
N1 Fe1 O11 123.91(14) . 5
N1 Fe1 O11 56.09(14) 5 5
N1 Fe1 O11 123.91(14) 3 5
N1 Fe1 O11 56.09(14) 7 5
N2 Fe1 O11 51.5(2) 5 5
N2 Fe1 O11 128.5(2) . 5
N1 Fe1 O11 56.09(14) . .
N1 Fe1 O11 123.91(14) 5 .
N1 Fe1 O11 56.09(14) 3 .
N1 Fe1 O11 123.91(14) 7 .
N2 Fe1 O11 128.5(2) 5 .
N2 Fe1 O11 51.5(2) . .
O11 Fe1 O11 180.0(5) 5 .
N1 Fe1 O11 56.09(14) . 5_655
N1 Fe1 O11 123.91(14) 5 5_655
N1 Fe1 O11 56.09(14) 3 5_655
N1 Fe1 O11 123.91(14) 7 5_655
N2 Fe1 O11 51.5(2) 5 5_655
N2 Fe1 O11 128.5(2) . 5_655
O11 Fe1 O11 103.0(5) 5 5_655
O11 Fe1 O11 77.0(5) . 5_655
N1 Fe1 O11 123.91(14) . 1_455
N1 Fe1 O11 56.09(14) 5 1_455
N1 Fe1 O11 123.91(14) 3 1_455
N1 Fe1 O11 56.09(14) 7 1_455
N2 Fe1 O11 128.5(2) 5 1_455
N2 Fe1 O11 51.5(2) . 1_455
O11 Fe1 O11 77.0(5) 5 1_455
O11 Fe1 O11 103.0(5) . 1_455
O11 Fe1 O11 180.0 5_655 1_455
O12 O10 O11 158.2(9) . .
O12 O10 O11 158.2(9) . 5_656
O11 O10 O11 43.6(18) . 5_656
O12 O10 O13 28.3(6) . 5_666
O11 O10 O13 144.8(7) . 5_666
O11 O10 O13 144.8(7) 5_656 5_666
O12 O10 O13 28.3(6) . .
O11 O10 O13 144.8(7) . .
O11 O10 O13 144.8(7) 5_656 .
O13 O10 O13 56.7(12) 5_666 .
O12 O10 O12 0.000(6) . 5_666
O11 O10 O12 158.2(9) . 5_666
O11 O10 O12 158.2(9) 5_656 5_666
O13 O10 O12 28.3(6) 5_666 5_666
O13 O10 O12 28.3(6) . 5_666
O12 O10 O10 180.000(5) . 5_656
O11 O10 O10 21.8(9) . 5_656
O11 O10 O10 21.8(9) 5_656 5_656
O13 O10 O10 151.7(6) 5_666 5_656
O13 O10 O10 151.7(6) . 5_656
O12 O10 O10 180.000(3) 5_666 5_656
O12 O10 C2 94.2(3) . .
O11 O10 C2 82.0(2) . .
O11 O10 C2 90.1(3) 5_656 .
O13 O10 C2 122.0(7) 5_666 .
O13 O10 C2 66.5(5) . .
O12 O10 C2 94.2(3) 5_666 .
O10 O10 C2 85.8(3) 5_656 .
O12 O10 C2 94.2(3) . 6_656
O11 O10 C2 90.1(3) . 6_656
O11 O10 C2 82.0(2) 5_656 6_656
O13 O10 C2 66.5(5) 5_666 6_656
O13 O10 C2 122.0(7) . 6_656
O12 O10 C2 94.2(3) 5_666 6_656
O10 O10 C2 85.8(3) 5_656 6_656
C2 O10 C2 171.5(5) . 6_656
O12 O10 C2 94.2(3) . 6_556
O11 O10 C2 90.1(3) . 6_556
O11 O10 C2 82.0(2) 5_656 6_556
O13 O10 C2 122.0(7) 5_666 6_556
O13 O10 C2 66.5(5) . 6_556
O12 O10 C2 94.2(3) 5_666 6_556
O10 O10 C2 85.8(3) 5_656 6_556
C2 O10 C2 22.11(9) . 6_556
C2 O10 C2 156.3(2) 6_656 6_556
O12 O10 C2 94.2(3) . 1_655
O11 O10 C2 82.0(2) . 1_655
O11 O10 C2 90.1(3) 5_656 1_655
O13 O10 C2 66.5(5) 5_666 1_655
O13 O10 C2 122.0(7) . 1_655
O12 O10 C2 94.2(3) 5_666 1_655
O10 O10 C2 85.8(3) 5_656 1_655
C2 O10 C2 156.3(2) . 1_655
C2 O10 C2 22.11(9) 6_656 1_655
C2 O10 C2 171.5(5) 6_556 1_655
O12 O10 C1 78.4(2) . 7_656
O11 O10 C1 121.7(9) . 7_656
O11 O10 C1 81.2(8) 5_656 7_656
O13 O10 C1 69.7(2) 5_666 7_656
O13 O10 C1 89.6(4) . 7_656
O12 O10 C1 78.4(2) 5_666 7_656
O10 O10 C1 101.6(2) 5_656 7_656
C2 O10 C1 122.73(8) . 7_656
C2 O10 C1 59.27(6) 6_656 7_656
C2 O10 C1 101.02(7) 6_556 7_656
C2 O10 C1 80.71(6) 1_655 7_656
O12 O10 C1 78.4(2) . .
O11 O10 C1 81.2(8) . .
O11 O10 C1 121.7(9) 5_656 .
O13 O10 C1 89.6(4) 5_666 .
O13 O10 C1 69.7(2) . .
O12 O10 C1 78.4(2) 5_666 .
O10 O10 C1 101.6(2) 5_656 .
C2 O10 C1 59.27(6) . .
C2 O10 C1 122.73(8) 6_656 .
C2 O10 C1 80.71(6) 6_556 .
C2 O10 C1 101.02(7) 1_655 .
C1 O10 C1 156.8(5) 7_656 .
O12 O10 C1 78.4(2) . 1_556
O11 O10 C1 121.7(9) . 1_556
O11 O10 C1 81.2(8) 5_656 1_556
O13 O10 C1 89.6(4) 5_666 1_556
O13 O10 C1 69.7(2) . 1_556
O12 O10 C1 78.4(2) 5_666 1_556
O10 O10 C1 101.6(2) 5_656 1_556
C2 O10 C1 80.71(6) . 1_556
C2 O10 C1 101.02(7) 6_656 1_556
C2 O10 C1 59.27(6) 6_556 1_556
C2 O10 C1 122.73(8) 1_655 1_556
C1 O10 C1 42.04(9) 7_656 1_556
C1 O10 C1 131.4(2) . 1_556
O12 O10 C1 78.4(2) . 7_655
O11 O10 C1 81.2(8) . 7_655
O11 O10 C1 121.7(9) 5_656 7_655
O13 O10 C1 69.7(2) 5_666 7_655
O13 O10 C1 89.6(4) . 7_655
O12 O10 C1 78.4(2) 5_666 7_655
O10 O10 C1 101.6(2) 5_656 7_655
C2 O10 C1 101.02(7) . 7_655
C2 O10 C1 80.71(6) 6_656 7_655
C2 O10 C1 122.73(8) 6_556 7_655
C2 O10 C1 59.27(6) 1_655 7_655
C1 O10 C1 131.4(2) 7_656 7_655
C1 O10 C1 42.04(9) . 7_655
C1 O10 C1 156.8(5) 1_556 7_655
O12 O10 Ni1 58.8(2) . 1_556
O11 O10 Ni1 143.0(10) . 1_556
O11 O10 Ni1 99.4(9) 5_656 1_556
O13 O10 Ni1 62.9(3) 5_666 1_556
O13 O10 Ni1 62.9(3) . 1_556
O12 O10 Ni1 58.8(2) 5_666 1_556
O10 O10 Ni1 121.2(2) 5_656 1_556
C2 O10 Ni1 101.67(14) . 1_556
C2 O10 Ni1 82.78(11) 6_656 1_556
C2 O10 Ni1 82.78(11) 6_556 1_556
C2 O10 Ni1 101.67(14) 1_655 1_556
C1 O10 Ni1 27.89(7) 7_656 1_556
C1 O10 Ni1 132.5(4) . 1_556
C1 O10 Ni1 27.89(7) 1_556 1_556
C1 O10 Ni1 132.5(4) 7_655 1_556
O12 O10 Ni1 58.8(2) . .
O11 O10 Ni1 99.4(9) . .
O11 O10 Ni1 143.0(10) 5_656 .
O13 O10 Ni1 62.9(3) 5_666 .
O13 O10 Ni1 62.9(3) . .
O12 O10 Ni1 58.8(2) 5_666 .
O10 O10 Ni1 121.2(2) 5_656 .
C2 O10 Ni1 82.78(11) . .
C2 O10 Ni1 101.67(14) 6_656 .
C2 O10 Ni1 101.67(14) 6_556 .
C2 O10 Ni1 82.78(11) 1_655 .
C1 O10 Ni1 132.5(4) 7_656 .
C1 O10 Ni1 27.89(7) . .
C1 O10 Ni1 132.5(4) 1_556 .
C1 O10 Ni1 27.89(7) 7_655 .
Ni1 O10 Ni1 117.6(4) 1_556 .
O12 O10 N1 90.6(2) . 7_656
O11 O10 N1 107.7(8) . 7_656
O11 O10 N1 71.2(7) 5_656 7_656
O13 O10 N1 75.7(3) 5_666 7_656
O13 O10 N1 105.3(4) . 7_656
O12 O10 N1 90.6(2) 5_666 7_656
O10 O10 N1 89.4(2) 5_656 7_656
C2 O10 N1 133.52(7) . 7_656
C2 O10 N1 46.37(5) 6_656 7_656
C2 O10 N1 111.45(6) 6_556 7_656
C2 O10 N1 68.46(5) 1_655 7_656
C1 O10 N1 16.45(6) 7_656 7_656
C1 O10 N1 164.4(3) . 7_656
C1 O10 N1 55.10(5) 1_556 7_656
C1 O10 N1 125.17(10) 7_655 7_656
Ni1 O10 N1 44.34(6) 1_556 7_656
Ni1 O10 N1 136.5(3) . 7_656
O12 O10 N1 90.6(2) . .
O11 O10 N1 71.2(7) . .
O11 O10 N1 107.7(8) 5_656 .
O13 O10 N1 105.3(4) 5_666 .
O13 O10 N1 75.7(3) . .
O12 O10 N1 90.6(2) 5_666 .
O10 O10 N1 89.4(2) 5_656 .
C2 O10 N1 46.37(5) . .
C2 O10 N1 133.52(7) 6_656 .
C2 O10 N1 68.46(5) 6_556 .
C2 O10 N1 111.45(6) 1_655 .
C1 O10 N1 164.4(3) 7_656 .
C1 O10 N1 16.45(6) . .
C1 O10 N1 125.17(10) 1_556 .
C1 O10 N1 55.10(5) 7_655 .
Ni1 O10 N1 136.5(3) 1_556 .
Ni1 O10 N1 44.34(6) . .
N1 O10 N1 178.9(5) 7_656 .
O12 O10 N1 90.6(2) . 7_655
O11 O10 N1 71.2(7) . 7_655
O11 O10 N1 107.7(8) 5_656 7_655
O13 O10 N1 75.7(3) 5_666 7_655
O13 O10 N1 105.3(4) . 7_655
O12 O10 N1 90.6(2) 5_666 7_655
O10 O10 N1 89.4(2) 5_656 7_655
C2 O10 N1 111.45(6) . 7_655
C2 O10 N1 68.46(5) 6_656 7_655
C2 O10 N1 133.52(7) 6_556 7_655
C2 O10 N1 46.37(5) 1_655 7_655
C1 O10 N1 125.17(10) 7_656 7_655
C1 O10 N1 55.10(5) . 7_655
C1 O10 N1 164.4(3) 1_556 7_655
C1 O10 N1 16.45(6) 7_655 7_655
Ni1 O10 N1 136.5(3) 1_556 7_655
Ni1 O10 N1 44.34(6) . 7_655
N1 O10 N1 114.71(6) 7_656 7_655
N1 O10 N1 65.28(6) . 7_655
O11 O11 O10 68.2(9) 5_656 .
O11 O11 O10 68.2(9) 5_656 5_656
O10 O11 O10 136.4(18) . 5_656
O11 O11 O12 78.9(5) 5_656 .
O10 O11 O12 10.7(5) . .
O10 O11 O12 147.0(14) 5_656 .
O11 O11 O12 78.9(5) 5_656 5_656
O10 O11 O12 147.0(14) . 5_656
O10 O11 O12 10.7(5) 5_656 5_656
O12 O11 O12 157.7(10) . 5_656
O11 O11 N2 103.3(4) 5_656 .
O10 O11 N2 94.91(8) . .
O10 O11 N2 94.91(8) 5_656 .
O12 O11 N2 92.55(5) . .
O12 O11 N2 92.55(5) 5_656 .
O11 O11 N2 103.3(4) 5_656 1_655
O10 O11 N2 94.91(8) . 1_655
O10 O11 N2 94.91(7) 5_656 1_655
O12 O11 N2 92.55(5) . 1_655
O12 O11 N2 92.55(5) 5_656 1_655
N2 O11 N2 153.4(8) . 1_655
O11 O11 O13 81.2(4) 5_656 5_666
O10 O11 O13 21.5(4) . 5_666
O10 O11 O13 144.8(11) 5_656 5_666
O12 O11 O13 17.6(4) . 5_666
O12 O11 O13 153.4(7) 5_656 5_666
N2 O11 O13 109.2(4) . 5_666
N2 O11 O13 75.0(4) 1_655 5_666
O11 O11 O13 81.2(4) 5_656 1_545
O10 O11 O13 144.8(11) . 1_545
O10 O11 O13 21.5(4) 5_656 1_545
O12 O11 O13 153.4(7) . 1_545
O12 O11 O13 17.6(4) 5_656 1_545
N2 O11 O13 75.0(4) . 1_545
N2 O11 O13 109.2(4) 1_655 1_545
O13 O11 O13 162.4(8) 5_666 1_545
O11 O11 O13 81.2(4) 5_656 .
O10 O11 O13 21.5(4) . .
O10 O11 O13 144.8(11) 5_656 .
O12 O11 O13 17.6(4) . .
O12 O11 O13 153.4(7) 5_656 .
N2 O11 O13 75.0(4) . .
N2 O11 O13 109.2(4) 1_655 .
O13 O11 O13 35.1(8) 5_666 .
O13 O11 O13 140.5(7) 1_545 .
O11 O11 O13 81.2(4) 5_656 5_656
O10 O11 O13 144.8(11) . 5_656
O10 O11 O13 21.5(4) 5_656 5_656
O12 O11 O13 153.4(7) . 5_656
O12 O11 O13 17.6(4) 5_656 5_656
N2 O11 O13 109.2(4) . 5_656
N2 O11 O13 75.0(4) 1_655 5_656
O13 O11 O13 140.5(7) 5_666 5_656
O13 O11 O13 35.1(8) 1_545 5_656
O13 O11 O13 162.4(8) . 5_656
O11 O11 C2 92.1(4) 5_656 2
O10 O11 C2 107.2(2) . 2
O10 O11 C2 74.43(6) 5_656 2
O12 O11 C2 107.75(10) . 2
O12 O11 C2 73.09(6) 5_656 2
N2 O11 C2 20.80(5) . 2
N2 O11 C2 156.7(5) 1_655 2
O13 O11 C2 125.3(4) 5_666 2
O13 O11 C2 55.4(4) 1_545 2
O13 O11 C2 90.2(4) . 2
O13 O11 C2 90.4(4) 5_656 2
O11 O11 C2 92.1(4) 5_656 1_655
O10 O11 C2 74.43(6) . 1_655
O10 O11 C2 107.2(2) 5_656 1_655
O12 O11 C2 73.09(6) . 1_655
O12 O11 C2 107.75(10) 5_656 1_655
N2 O11 C2 156.7(5) . 1_655
N2 O11 C2 20.80(5) 1_655 1_655
O13 O11 C2 55.4(4) 5_666 1_655
O13 O11 C2 125.3(4) 1_545 1_655
O13 O11 C2 90.4(4) . 1_655
O13 O11 C2 90.2(4) 5_656 1_655
C2 O11 C2 175.9(8) 2 1_655
O11 O11 C2 92.1(4) 5_656 2_655
O10 O11 C2 107.2(2) . 2_655
O10 O11 C2 74.43(6) 5_656 2_655
O12 O11 C2 107.75(10) . 2_655
O12 O11 C2 73.09(6) 5_656 2_655
N2 O11 C2 156.7(5) . 2_655
N2 O11 C2 20.80(5) 1_655 2_655
O13 O11 C2 90.2(4) 5_666 2_655
O13 O11 C2 90.4(4) 1_545 2_655
O13 O11 C2 125.3(4) . 2_655
O13 O11 C2 55.4(4) 5_656 2_655
C2 O11 C2 144.39(13) 2 2_655
C2 O11 C2 35.35(9) 1_655 2_655
O11 O11 C2 92.1(4) 5_656 .
O10 O11 C2 74.43(6) . .
O10 O11 C2 107.2(2) 5_656 .
O12 O11 C2 73.09(6) . .
O12 O11 C2 107.75(10) 5_656 .
N2 O11 C2 20.80(5) . .
N2 O11 C2 156.7(5) 1_655 .
O13 O11 C2 90.4(4) 5_666 .
O13 O11 C2 90.2(4) 1_545 .
O13 O11 C2 55.4(4) . .
O13 O11 C2 125.3(4) 5_656 .
C2 O11 C2 35.35(9) 2 .
C2 O11 C2 144.39(13) 1_655 .
C2 O11 C2 175.9(8) 2_655 .
O11 O11 C1 138.2(2) 5_656 3
O10 O11 C1 143.4(9) . 3
O10 O11 C1 75.6(6) 5_656 3
O12 O11 C1 134.4(6) . 3
O12 O11 C1 65.7(3) 5_656 3
N2 O11 C1 59.1(2) . 3
N2 O11 C1 99.8(4) 1_655 3
O13 O11 C1 138.9(6) 5_666 3
O13 O11 C1 58.32(17) 1_545 3
O13 O11 C1 122.8(5) . 3
O13 O11 C1 71.7(3) 5_656 3
C2 O11 C1 57.75(18) 2 3
C2 O11 C1 118.7(5) 1_655 3
C2 O11 C1 97.8(3) 2_655 3
C2 O11 C1 79.1(3) . 3
O11 O11 C1 138.2(3) 5_656 5_655
O10 O11 C1 143.4(9) . 5_655
O10 O11 C1 75.6(6) 5_656 5_655
O12 O11 C1 134.4(6) . 5_655
O12 O11 C1 65.7(3) 5_656 5_655
N2 O11 C1 99.8(4) . 5_655
N2 O11 C1 59.1(2) 1_655 5_655
O13 O11 C1 122.8(5) 5_666 5_655
O13 O11 C1 71.7(3) 1_545 5_655
O13 O11 C1 138.9(6) . 5_655
O13 O11 C1 58.32(17) 5_656 5_655
C2 O11 C1 97.8(3) 2 5_655
C2 O11 C1 79.1(3) 1_655 5_655
C2 O11 C1 57.75(18) 2_655 5_655
C2 O11 C1 118.7(5) . 5_655
C1 O11 C1 41.2(2) 3 5_655
O11 O11 C1 138.2(3) 5_656 .
O10 O11 C1 75.6(6) . .
O10 O11 C1 143.4(9) 5_656 .
O12 O11 C1 65.7(3) . .
O12 O11 C1 134.4(6) 5_656 .
N2 O11 C1 59.1(2) . .
N2 O11 C1 99.8(4) 1_655 .
O13 O11 C1 71.7(3) 5_666 .
O13 O11 C1 122.8(5) 1_545 .
O13 O11 C1 58.32(17) . .
O13 O11 C1 138.9(6) 5_656 .
C2 O11 C1 79.1(3) 2 .
C2 O11 C1 97.8(3) 1_655 .
C2 O11 C1 118.7(5) 2_655 .
C2 O11 C1 57.75(18) . .
C1 O11 C1 69.0(4) 3 .
C1 O11 C1 83.6(5) 5_655 .
O11 O11 C1 138.2(3) 5_656 7_655
O10 O11 C1 75.6(6) . 7_655
O10 O11 C1 143.4(9) 5_656 7_655
O12 O11 C1 65.7(3) . 7_655
O12 O11 C1 134.4(6) 5_656 7_655
N2 O11 C1 99.8(4) . 7_655
N2 O11 C1 59.1(2) 1_655 7_655
O13 O11 C1 58.32(17) 5_666 7_655
O13 O11 C1 138.9(6) 1_545 7_655
O13 O11 C1 71.7(3) . 7_655
O13 O11 C1 122.8(5) 5_656 7_655
C2 O11 C1 118.7(5) 2 7_655
C2 O11 C1 57.75(18) 1_655 7_655
C2 O11 C1 79.1(3) 2_655 7_655
C2 O11 C1 97.8(3) . 7_655
C1 O11 C1 83.6(5) 3 7_655
C1 O11 C1 69.0(4) 5_655 7_655
C1 O11 C1 41.2(2) . 7_655
O11 O11 N1 137.8(2) 5_656 3
O10 O11 N1 127.4(7) . 3
O10 O11 N1 86.8(6) 5_656 3
O12 O11 N1 119.6(4) . 3
O12 O11 N1 78.0(3) 5_656 3
N2 O11 N1 43.60(17) . 3
N2 O11 N1 112.5(6) 1_655 3
O13 O11 N1 128.4(5) 5_666 3
O13 O11 N1 66.8(3) 1_545 3
O13 O11 N1 106.1(4) . 3
O13 O11 N1 87.1(3) 5_656 3
C2 O11 N1 47.41(14) 2 3
C2 O11 N1 128.6(6) 1_655 3
C2 O11 N1 114.0(5) 2_655 3
C2 O11 N1 62.62(19) . 3
C1 O11 N1 17.36(11) 3 3
C1 O11 N1 56.3(3) 5_655 3
C1 O11 N1 56.7(3) . 3
C1 O11 N1 81.4(5) 7_655 3
O12 O12 O13 61.5(15) 5_666 5_666
O12 O12 O13 61.5(15) 5_666 .
O13 O12 O13 123(3) 5_666 .
O12 O12 O10 180.000(7) 5_666 .
O13 O12 O10 118.5(15) 5_666 .
O13 O12 O10 118.5(15) . .
O12 O12 O10 0.000(6) 5_666 5_666
O13 O12 O10 61.5(15) 5_666 5_666
O13 O12 O10 61.5(15) . 5_666
O10 O12 O10 180.000(2) . 5_666
O12 O12 O11 168.9(5) 5_666 .
O13 O12 O11 117.9(15) 5_666 .
O13 O12 O11 117.9(15) . .
O10 O12 O11 11.1(5) . .
O10 O12 O11 168.9(5) 5_666 .
O12 O12 O11 168.9(5) 5_666 5_656
O13 O12 O11 117.9(15) 5_666 5_656
O13 O12 O11 117.9(15) . 5_656
O10 O12 O11 11.1(5) . 5_656
O10 O12 O11 168.9(5) 5_666 5_656
O11 O12 O11 22.3(10) . 5_656
O12 O12 Ni1 79.9(6) 5_666 1_556
O13 O12 Ni1 85.2(5) 5_666 1_556
O13 O12 Ni1 85.2(5) . 1_556
O10 O12 Ni1 100.1(6) . 1_556
O10 O12 Ni1 79.9(6) 5_666 1_556
O11 O12 Ni1 111.2(8) . 1_556
O11 O12 Ni1 88.9(6) 5_656 1_556
O12 O12 Ni1 79.9(6) 5_666 .
O13 O12 Ni1 85.2(5) 5_666 .
O13 O12 Ni1 85.2(5) . .
O10 O12 Ni1 100.1(6) . .
O10 O12 Ni1 79.9(6) 5_666 .
O11 O12 Ni1 88.9(6) . .
O11 O12 Ni1 111.2(8) 5_656 .
Ni1 O12 Ni1 159.9(11) 1_556 .
O12 O12 C1 100.9(5) 5_666 .
O13 O12 C1 114.0(2) 5_666 .
O13 O12 C1 77.0(3) . .
O10 O12 C1 79.1(5) . .
O10 O12 C1 100.9(5) 5_666 .
O11 O12 C1 68.7(6) . .
O11 O12 C1 89.4(8) 5_656 .
Ni1 O12 C1 158.86(6) 1_556 .
Ni1 O12 C1 29.95(5) . .
O12 O12 C1 100.9(5) 5_666 7_656
O13 O12 C1 77.0(3) 5_666 7_656
O13 O12 C1 114.0(2) . 7_656
O10 O12 C1 79.1(5) . 7_656
O10 O12 C1 100.9(5) 5_666 7_656
O11 O12 C1 89.4(8) . 7_656
O11 O12 C1 68.7(6) 5_656 7_656
Ni1 O12 C1 29.95(5) 1_556 7_656
Ni1 O12 C1 158.86(6) . 7_656
C1 O12 C1 158.1(10) . 7_656
O12 O12 C1 100.9(5) 5_666 7_655
O13 O12 C1 77.0(3) 5_666 7_655
O13 O12 C1 114.0(2) . 7_655
O10 O12 C1 79.1(5) . 7_655
O10 O12 C1 100.9(5) 5_666 7_655
O11 O12 C1 68.7(6) . 7_655
O11 O12 C1 89.4(8) 5_656 7_655
Ni1 O12 C1 158.86(6) 1_556 7_655
Ni1 O12 C1 29.95(5) . 7_655
C1 O12 C1 42.14(11) . 7_655
C1 O12 C1 132.0(5) 7_656 7_655
O12 O12 C1 100.9(5) 5_666 1_556
O13 O12 C1 114.0(2) 5_666 1_556
O13 O12 C1 77.0(3) . 1_556
O10 O12 C1 79.1(5) . 1_556
O10 O12 C1 100.9(5) 5_666 1_556
O11 O12 C1 89.4(8) . 1_556
O11 O12 C1 68.7(6) 5_656 1_556
Ni1 O12 C1 29.95(5) 1_556 1_556
Ni1 O12 C1 158.86(6) . 1_556
C1 O12 C1 132.0(5) . 1_556
C1 O12 C1 42.14(11) 7_656 1_556
C1 O12 C1 158.1(10) 7_655 1_556
O12 O12 C2 115.4(4) 5_666 .
O13 O12 C2 169.6(5) 5_666 .
O13 O12 C2 54.9(11) . .
O10 O12 C2 64.6(4) . .
O10 O12 C2 115.4(4) 5_666 .
O11 O12 C2 63.0(4) . .
O11 O12 C2 67.2(5) 5_656 .
Ni1 O12 C2 104.23(19) 1_556 .
Ni1 O12 C2 84.48(16) . .
C1 O12 C2 56.03(19) . .
C1 O12 C2 113.3(5) 7_656 .
C1 O12 C2 94.5(3) 7_655 .
C1 O12 C2 76.0(3) 1_556 .
O12 O12 C2 115.4(4) 5_666 6_556
O13 O12 C2 169.6(5) 5_666 6_556
O13 O12 C2 54.9(11) . 6_556
O10 O12 C2 64.6(4) . 6_556
O10 O12 C2 115.4(4) 5_666 6_556
O11 O12 C2 67.2(5) . 6_556
O11 O12 C2 63.0(4) 5_656 6_556
Ni1 O12 C2 84.48(16) 1_556 6_556
Ni1 O12 C2 104.23(19) . 6_556
C1 O12 C2 76.0(3) . 6_556
C1 O12 C2 94.5(3) 7_656 6_556
C1 O12 C2 113.3(5) 7_655 6_556
C1 O12 C2 56.03(19) 1_556 6_556
C2 O12 C2 20.00(10) . 6_556
O12 O12 C2 115.4(4) 5_666 6_656
O13 O12 C2 54.9(11) 5_666 6_656
O13 O12 C2 169.6(5) . 6_656
O10 O12 C2 64.6(4) . 6_656
O10 O12 C2 115.4(4) 5_666 6_656
O11 O12 C2 67.2(5) . 6_656
O11 O12 C2 63.0(4) 5_656 6_656
Ni1 O12 C2 84.48(16) 1_556 6_656
Ni1 O12 C2 104.23(19) . 6_656
C1 O12 C2 113.3(5) . 6_656
C1 O12 C2 56.03(19) 7_656 6_656
C1 O12 C2 76.0(3) 7_655 6_656
C1 O12 C2 94.5(3) 1_556 6_656
C2 O12 C2 129.2(9) . 6_656
C2 O12 C2 124.9(8) 6_556 6_656
O12 O12 C2 115.4(4) 5_666 1_655
O13 O12 C2 54.9(11) 5_666 1_655
O13 O12 C2 169.6(5) . 1_655
O10 O12 C2 64.6(4) . 1_655
O10 O12 C2 115.4(4) 5_666 1_655
O11 O12 C2 63.0(4) . 1_655
O11 O12 C2 67.2(5) 5_656 1_655
Ni1 O12 C2 104.23(19) 1_556 1_655
Ni1 O12 C2 84.48(16) . 1_655
C1 O12 C2 94.5(3) . 1_655
C1 O12 C2 76.0(3) 7_656 1_655
C1 O12 C2 56.03(19) 7_655 1_655
C1 O12 C2 113.3(5) 1_556 1_655
C2 O12 C2 124.9(8) . 1_655
C2 O12 C2 129.2(9) 6_556 1_655
C2 O12 C2 20.00(10) 6_656 1_655
O12 O12 O11 7.9(4) 5_666 5_666
O13 O12 O11 61.8(15) 5_666 5_666
O13 O12 O11 61.8(15) . 5_666
O10 O12 O11 172.1(4) . 5_666
O10 O12 O11 7.9(4) 5_666 5_666
O11 O12 O11 176.8(2) . 5_666
O11 O12 O11 161.0(8) 5_656 5_666
Ni1 O12 O11 72.1(6) 1_556 5_666
Ni1 O12 O11 87.8(7) . 5_666
C1 O12 O11 108.3(7) . 5_666
C1 O12 O11 93.6(6) 7_656 5_666
C1 O12 O11 108.3(7) 7_655 5_666
C1 O12 O11 93.6(6) 1_556 5_666
C2 O12 O11 116.7(4) . 5_666
C2 O12 O11 113.6(4) 6_556 5_666
C2 O12 O11 113.6(4) 6_656 5_666
C2 O12 O11 116.7(4) 1_655 5_666
O12 O12 O11 7.9(4) 5_666 1_565
O13 O12 O11 61.8(15) 5_666 1_565
O13 O12 O11 61.8(15) . 1_565
O10 O12 O11 172.1(4) . 1_565
O10 O12 O11 7.9(4) 5_666 1_565
O11 O12 O11 161.0(8) . 1_565
O11 O12 O11 176.8(2) 5_656 1_565
Ni1 O12 O11 87.8(7) 1_556 1_565
Ni1 O12 O11 72.1(6) . 1_565
C1 O12 O11 93.6(6) . 1_565
C1 O12 O11 108.3(7) 7_656 1_565
C1 O12 O11 93.6(6) 7_655 1_565
C1 O12 O11 108.3(7) 1_556 1_565
C2 O12 O11 113.6(4) . 1_565
C2 O12 O11 116.7(4) 6_556 1_565
C2 O12 O11 116.7(4) 6_656 1_565
C2 O12 O11 113.6(4) 1_655 1_565
O11 O12 O11 15.8(7) 5_666 1_565
O12 O12 C1 62.4(4) 5_666 5_666
O13 O12 C1 59.6(6) 5_666 5_666
O13 O12 C1 93.7(11) . 5_666
O10 O12 C1 117.6(4) . 5_666
O10 O12 C1 62.4(4) 5_666 5_666
O11 O12 C1 127.9(7) . 5_666
O11 O12 C1 107.2(5) 5_656 5_666
Ni1 O12 C1 26.78(14) 1_556 5_666
Ni1 O12 C1 137.0(8) . 5_666
C1 O12 C1 163.3(9) . 5_666
C1 O12 C1 38.56(12) 7_656 5_666
C1 O12 C1 136.4(4) 7_655 5_666
C1 O12 C1 56.73(13) 1_556 5_666
C2 O12 C1 129.02(7) . 5_666
C2 O12 C1 110.08(6) 6_556 5_666
C2 O12 C1 76.58(6) 6_656 5_666
C2 O12 C1 93.11(6) 1_655 5_666
O11 O12 C1 55.1(5) 5_666 5_666
O11 O12 C1 69.8(6) 1_565 5_666
O12 O13 O12 57(3) 5_666 .
O12 O13 O13 28.5(15) 5_666 5_666
O12 O13 O13 28.5(15) . 5_666
O12 O13 O10 33.2(14) 5_666 5_666
O12 O13 O10 90.2(19) . 5_666
O13 O13 O10 61.7(6) 5_666 5_666
O12 O13 O10 90.2(19) 5_666 .
O12 O13 O10 33.2(14) . .
O13 O13 O10 61.7(6) 5_666 .
O10 O13 O10 123.3(12) 5_666 .
O12 O13 C2 161.1(13) 5_666 .
O12 O13 C2 107.7(14) . .
O13 O13 C2 135.3(3) 5_666 .
O10 O13 C2 158.5(7) 5_666 .
O10 O13 C2 75.2(3) . .
O12 O13 C2 161.1(13) 5_666 6_556
O12 O13 C2 107.7(14) . 6_556
O13 O13 C2 135.3(3) 5_666 6_556
O10 O13 C2 158.5(7) 5_666 6_556
O10 O13 C2 75.2(3) . 6_556
C2 O13 C2 23.33(15) . 6_556
O12 O13 C2 107.7(14) 5_666 5_566
O12 O13 C2 161.1(13) . 5_566
O13 O13 C2 135.3(3) 5_666 5_566
O10 O13 C2 75.2(3) 5_666 5_566
O10 O13 C2 158.5(7) . 5_566
C2 O13 C2 89.4(6) . 5_566
C2 O13 C2 84.7(6) 6_556 5_566
O12 O13 C2 107.7(14) 5_666 2_565
O12 O13 C2 161.1(13) . 2_565
O13 O13 C2 135.3(3) 5_666 2_565
O10 O13 C2 75.2(3) 5_666 2_565
O10 O13 C2 158.5(7) . 2_565
C2 O13 C2 84.7(6) . 2_565
C2 O13 C2 89.4(6) 6_556 2_565
C2 O13 C2 23.33(15) 5_566 2_565
O12 O13 Ni1 74.2(5) 5_666 1_556
O12 O13 Ni1 74.2(5) . 1_556
O13 O13 Ni1 71.9(4) 5_666 1_556
O10 O13 Ni1 81.5(3) 5_666 1_556
O10 O13 Ni1 81.5(3) . 1_556
C2 O13 Ni1 114.4(3) . 1_556
C2 O13 Ni1 91.63(17) 6_556 1_556
C2 O13 Ni1 91.63(17) 5_566 1_556
C2 O13 Ni1 114.4(3) 2_565 1_556
O12 O13 Ni1 74.2(5) 5_666 .
O12 O13 Ni1 74.2(5) . .
O13 O13 Ni1 71.9(4) 5_666 .
O10 O13 Ni1 81.5(3) 5_666 .
O10 O13 Ni1 81.5(3) . .
C2 O13 Ni1 91.63(17) . .
C2 O13 Ni1 114.4(3) 6_556 .
C2 O13 Ni1 114.4(3) 5_566 .
C2 O13 Ni1 91.63(17) 2_565 .
Ni1 O13 Ni1 143.8(8) 1_556 .
O12 O13 C1 103.1(7) 5_666 .
O12 O13 C1 83.3(5) . .
O13 O13 C1 93.6(4) 5_666 .
O10 O13 C1 110.2(3) 5_666 .
O10 O13 C1 73.38(10) . .
C2 O13 C1 61.69(19) . .
C2 O13 C1 84.4(3) 6_556 .
C2 O13 C1 112.7(5) 5_566 .
C2 O13 C1 90.5(3) 2_565 .
Ni1 O13 C1 154.8(5) 1_556 .
Ni1 O13 C1 30.00(5) . .
O12 O13 C1 83.3(5) 5_666 3_566
O12 O13 C1 103.1(7) . 3_566
O13 O13 C1 93.6(4) 5_666 3_566
O10 O13 C1 73.38(10) 5_666 3_566
O10 O13 C1 110.2(3) . 3_566
C2 O13 C1 112.7(5) . 3_566
C2 O13 C1 90.5(3) 6_556 3_566
C2 O13 C1 61.69(19) 5_566 3_566
C2 O13 C1 84.4(3) 2_565 3_566
Ni1 O13 C1 30.00(5) 1_556 3_566
Ni1 O13 C1 154.8(5) . 3_566
C1 O13 C1 172.8(8) . 3_566
O12 O13 C1 83.3(5) 5_666 3_565
O12 O13 C1 103.1(7) . 3_565
O13 O13 C1 93.6(4) 5_666 3_565
O10 O13 C1 73.38(10) 5_666 3_565
O10 O13 C1 110.2(3) . 3_565
C2 O13 C1 90.5(3) . 3_565
C2 O13 C1 112.7(5) 6_556 3_565
C2 O13 C1 84.4(3) 5_566 3_565
C2 O13 C1 61.69(19) 2_565 3_565
Ni1 O13 C1 154.8(5) 1_556 3_565
Ni1 O13 C1 30.00(5) . 3_565
C1 O13 C1 42.03(9) . 3_565
C1 O13 C1 137.31(16) 3_566 3_565
O12 O13 C1 103.1(7) 5_666 1_556
O12 O13 C1 83.3(5) . 1_556
O13 O13 C1 93.6(4) 5_666 1_556
O10 O13 C1 110.2(3) 5_666 1_556
O10 O13 C1 73.38(10) . 1_556
C2 O13 C1 84.4(3) . 1_556
C2 O13 C1 61.69(19) 6_556 1_556
C2 O13 C1 90.5(3) 5_566 1_556
C2 O13 C1 112.7(5) 2_565 1_556
Ni1 O13 C1 30.00(5) 1_556 1_556
Ni1 O13 C1 154.8(5) . 1_556
C1 O13 C1 137.31(16) . 1_556
C1 O13 C1 42.03(9) 3_566 1_556
C1 O13 C1 172.8(8) 3_565 1_556
O12 O13 O11 44.4(14) 5_666 5_666
O12 O13 O11 100.6(17) . 5_666
O13 O13 O11 72.5(4) 5_666 5_666
O10 O13 O11 13.7(3) 5_666 5_666
O10 O13 O11 133.3(9) . 5_666
C2 O13 O11 151.5(7) . 5_666
C2 O13 O11 144.8(6) 6_556 5_666
C2 O13 O11 63.22(11) 5_566 5_666
C2 O13 O11 67.13(15) 2_565 5_666
Ni1 O13 O11 76.2(4) 1_556 5_666
Ni1 O13 O11 93.0(5) . 5_666
C1 O13 O11 119.9(4) . 5_666
C1 O13 O11 62.5(4) 3_566 5_666
C1 O13 O11 79.9(4) 3_565 5_666
C1 O13 O11 102.3(4) 1_556 5_666
O12 O13 O11 44.4(14) 5_666 1_565
O12 O13 O11 100.6(17) . 1_565
O13 O13 O11 72.5(4) 5_666 1_565
O10 O13 O11 13.7(3) 5_666 1_565
O10 O13 O11 133.3(9) . 1_565
C2 O13 O11 144.8(6) . 1_565
C2 O13 O11 151.5(7) 6_556 1_565
C2 O13 O11 67.13(15) 5_566 1_565
C2 O13 O11 63.22(11) 2_565 1_565
Ni1 O13 O11 93.0(5) 1_556 1_565
Ni1 O13 O11 76.2(4) . 1_565
C1 O13 O11 102.3(4) . 1_565
C1 O13 O11 79.9(4) 3_566 1_565
C1 O13 O11 62.5(4) 3_565 1_565
C1 O13 O11 119.9(4) 1_556 1_565
O11 O13 O11 17.6(8) 5_666 1_565
O12 O13 O11 100.6(17) 5_666 .
O12 O13 O11 44.4(14) . .
O13 O13 O11 72.5(4) 5_666 .
O10 O13 O11 133.3(9) 5_666 .
O10 O13 O11 13.7(3) . .
C2 O13 O11 63.22(11) . .
C2 O13 O11 67.13(15) 6_556 .
C2 O13 O11 151.5(7) 5_566 .
C2 O13 O11 144.8(6) 2_565 .
Ni1 O13 O11 93.0(5) 1_556 .
Ni1 O13 O11 76.2(4) . .
C1 O13 O11 62.5(4) . .
C1 O13 O11 119.9(4) 3_566 .
C1 O13 O11 102.3(4) 3_565 .
C1 O13 O11 79.9(4) 1_556 .
O11 O13 O11 144.9(8) 5_666 .
O11 O13 O11 140.5(7) 1_565 .
O12 O13 O11 100.6(17) 5_666 5_656
O12 O13 O11 44.4(14) . 5_656
O13 O13 O11 72.5(4) 5_666 5_656
O10 O13 O11 133.3(9) 5_666 5_656
O10 O13 O11 13.7(3) . 5_656
C2 O13 O11 67.13(15) . 5_656
C2 O13 O11 63.22(11) 6_556 5_656
C2 O13 O11 144.8(6) 5_566 5_656
C2 O13 O11 151.5(7) 2_565 5_656
Ni1 O13 O11 76.2(4) 1_556 5_656
Ni1 O13 O11 93.0(5) . 5_656
C1 O13 O11 79.9(4) . 5_656
C1 O13 O11 102.3(4) 3_566 5_656
C1 O13 O11 119.9(4) 3_565 5_656
C1 O13 O11 62.5(4) 1_556 5_656
O11 O13 O11 140.5(7) 5_666 5_656
O11 O13 O11 144.9(8) 1_565 5_656
O11 O13 O11 17.6(8) . 5_656
O12 O13 N1 118.0(7) 5_666 .
O12 O13 N1 89.1(8) . .
O13 O13 N1 105.0(3) 5_666 .
O10 O13 N1 124.69(15) 5_666 .
O10 O13 N1 71.10(12) . .
C2 O13 N1 46.25(14) . .
C2 O13 N1 69.0(2) 6_556 .
C2 O13 N1 108.9(5) 5_566 .
C2 O13 N1 89.5(4) 2_565 .
Ni1 O13 N1 149.51(8) 1_556 .
Ni1 O13 N1 45.46(4) . .
C1 O13 N1 15.46(8) . .
C1 O13 N1 158.7(6) 3_566 .
C1 O13 N1 53.13(8) 3_565 .
C1 O13 N1 124.6(2) 1_556 .
O11 O13 N1 132.9(4) 5_666 .
O11 O13 N1 115.4(4) 1_565 .
O11 O13 N1 58.3(3) . .
O11 O13 N1 74.1(4) 5_656 .
C1 N1 Fe1 178.7(3) . .
C1 N1 O11 80.21(14) . .
Fe1 N1 O11 98.90(8) . .
C1 N1 O11 80.21(14) . 5_655
Fe1 N1 O11 98.90(8) . 5_655
O11 N1 O11 95.6(5) . 5_655
C1 N1 O10 66.43(19) . .
Fe1 N1 O10 113.03(18) . .
O11 N1 O10 22.0(3) . .
O11 N1 O10 108.7(3) 5_655 .
C1 N1 O10 66.43(19) . 1_554
Fe1 N1 O10 113.03(18) . 1_554
O11 N1 O10 108.7(3) . 1_554
O11 N1 O10 22.0(3) 5_655 1_554
O10 N1 O10 114.71(6) . 1_554
C1 N1 O13 57.6(3) . .
Fe1 N1 O13 122.7(2) . .
O11 N1 O13 54.9(3) . .
O11 N1 O13 130.1(4) 5_655 .
O10 N1 O13 33.2(3) . .
O10 N1 O13 123.2(3) 1_554 .
C1 N1 O13 57.6(3) . 1_554
Fe1 N1 O13 122.7(2) . 1_554
O11 N1 O13 130.1(4) . 1_554
O11 N1 O13 54.9(3) 5_655 1_554
O10 N1 O13 123.2(3) . 1_554
O10 N1 O13 33.2(3) 1_554 1_554
O13 N1 O13 110.6(3) . 1_554
C2 N2 C2 116.1(3) . 2
C2 N2 Fe1 121.94(17) . .
C2 N2 Fe1 121.94(17) 2 .
C2 N2 O11 83.0(2) . .
C2 N2 O11 83.0(2) 2 .
Fe1 N2 O11 103.3(4) . .
C2 N2 O11 83.0(2) . 1_455
C2 N2 O11 83.0(2) 2 1_455
Fe1 N2 O11 103.3(4) . 1_455
O11 N2 O11 153.4(8) . 1_455
C2 N2 O11 75.18(17) . 5_656
C2 N2 O11 75.18(17) 2 5_656
Fe1 N2 O11 118.9(3) . 5_656
O11 N2 O11 15.6(7) . 5_656
O11 N2 O11 137.76(12) 1_455 5_656
C2 N2 O11 75.18(17) . 5_556
C2 N2 O11 75.18(17) 2 5_556
Fe1 N2 O11 118.9(3) . 5_556
O11 N2 O11 137.76(12) . 5_556
O11 N2 O11 15.6(7) 1_455 5_556
O11 N2 O11 122.1(6) 5_656 5_556
C2 N2 O10 61.66(18) . .
C2 N2 O10 96.3(2) 2 .
Fe1 N2 O10 110.16(5) . .
O11 N2 O10 21.7(2) . .
O11 N2 O10 140.4(3) 1_455 .
O11 N2 O10 21.4(2) 5_656 .
O11 N2 O10 126.7(3) 5_556 .
C2 N2 O10 96.3(2) . 5_556
C2 N2 O10 61.66(18) 2 5_556
Fe1 N2 O10 110.16(5) . 5_556
O11 N2 O10 140.4(3) . 5_556
O11 N2 O10 21.7(2) 1_455 5_556
O11 N2 O10 126.7(3) 5_656 5_556
O11 N2 O10 21.4(2) 5_556 5_556
O10 N2 O10 139.68(11) . 5_556
C2 N2 O10 96.3(2) . 5_656
C2 N2 O10 61.66(18) 2 5_656
Fe1 N2 O10 110.16(5) . 5_656
O11 N2 O10 21.7(2) . 5_656
O11 N2 O10 140.4(3) 1_455 5_656
O11 N2 O10 21.4(2) 5_656 5_656
O11 N2 O10 126.7(3) 5_556 5_656
O10 N2 O10 40.3(4) . 5_656
O10 N2 O10 121.7(3) 5_556 5_656
C2 N2 O10 61.66(18) . 1_455
C2 N2 O10 96.3(2) 2 1_455
Fe1 N2 O10 110.16(5) . 1_455
O11 N2 O10 140.4(3) . 1_455
O11 N2 O10 21.7(2) 1_455 1_455
O11 N2 O10 126.7(3) 5_656 1_455
O11 N2 O10 21.4(2) 5_556 1_455
O10 N2 O10 121.7(3) . 1_455
O10 N2 O10 40.3(4) 5_556 1_455
O10 N2 O10 139.68(11) 5_656 1_455
N1 C1 Ni1 178.8(3) . .
N1 C1 O13 106.9(3) . .
Ni1 C1 O13 72.8(3) . .
N1 C1 O13 106.9(3) . 1_554
Ni1 C1 O13 72.8(3) . 1_554
O13 C1 O13 137.31(16) . 1_554
N1 C1 O12 113.1(4) . .
Ni1 C1 O12 67.1(4) . .
O13 C1 O12 19.7(4) . .
O13 C1 O12 139.5(5) 1_554 .
N1 C1 O12 113.1(4) . 1_554
Ni1 C1 O12 67.1(4) . 1_554
O13 C1 O12 139.5(5) . 1_554
O13 C1 O12 19.7(4) 1_554 1_554
O12 C1 O12 132.0(5) . 1_554
N1 C1 O10 97.1(2) . .
Ni1 C1 O10 83.34(19) . .
O13 C1 O10 36.9(3) . .
O13 C1 O10 154.0(4) 1_554 .
O12 C1 O10 22.5(6) . .
O12 C1 O10 137.90(9) 1_554 .
N1 C1 O10 97.1(2) . 1_554
Ni1 C1 O10 83.34(19) . 1_554
O13 C1 O10 154.0(4) . 1_554
O13 C1 O10 36.9(3) 1_554 1_554
O12 C1 O10 137.90(9) . 1_554
O12 C1 O10 22.5(6) 1_554 1_554
O10 C1 O10 131.4(2) . 1_554
N1 C1 O11 82.43(14) . 5_655
Ni1 C1 O11 98.34(8) . 5_655
O13 C1 O11 151.1(4) . 5_655
O13 C1 O11 59.1(3) 1_554 5_655
O12 C1 O11 131.5(4) . 5_655
O12 C1 O11 45.6(6) 1_554 5_655
O10 C1 O11 116.1(3) . 5_655
O10 C1 O11 23.2(3) 1_554 5_655
N1 C1 O11 82.43(14) . .
Ni1 C1 O11 98.34(8) . .
O13 C1 O11 59.1(3) . .
O13 C1 O11 151.1(4) 1_554 .
O12 C1 O11 45.6(6) . .
O12 C1 O11 131.5(4) 1_554 .
O10 C1 O11 23.2(3) . .
O10 C1 O11 116.1(3) 1_554 .
O11 C1 O11 96.4(5) 5_655 .
N1 C1 O12 123.6(2) . 5_666
Ni1 C1 O12 56.2(3) . 5_666
O13 C1 O12 17.4(4) . 5_666
O13 C1 O12 125.6(4) 1_554 5_666
O12 C1 O12 16.7(9) . 5_666
O12 C1 O12 123.27(13) 1_554 5_666
O10 C1 O12 39.2(5) . 5_666
O10 C1 O12 136.75(16) 1_554 5_666
O11 C1 O12 139.7(2) 5_655 5_666
O11 C1 O12 62.2(5) . 5_666
N1 C1 O12 123.6(2) . 5_665
Ni1 C1 O12 56.2(3) . 5_665
O13 C1 O12 125.6(4) . 5_665
O13 C1 O12 17.4(4) 1_554 5_665
O12 C1 O12 123.27(13) . 5_665
O12 C1 O12 16.7(9) 1_554 5_665
O10 C1 O12 136.75(16) . 5_665
O10 C1 O12 39.2(5) 1_554 5_665
O11 C1 O12 62.2(5) 5_655 5_665
O11 C1 O12 139.7(2) . 5_665
O12 C1 O12 111.1(6) 5_666 5_665
N2 C2 C2 121.94(17) . 6_556
N2 C2 O13 132.7(3) . .
C2 C2 O13 78.33(8) 6_556 .
N2 C2 O13 132.7(3) . 5_566
C2 C2 O13 78.33(8) 6_556 5_566
O13 C2 O13 90.6(6) . 5_566
N2 C2 O10 99.5(2) . .
C2 C2 O10 78.95(4) 6_556 .
O13 C2 O10 38.3(4) . .
O13 C2 O10 127.4(4) 5_566 .
N2 C2 O10 99.5(2) . 1_455
C2 C2 O10 78.95(4) 6_556 1_455
O13 C2 O10 127.4(4) . 1_455
O13 C2 O10 38.3(4) 5_566 1_455
O10 C2 O10 156.3(2) . 1_455
N2 C2 O11 76.2(2) . 1_455
C2 C2 O11 87.9(4) 6_556 1_455
O13 C2 O11 150.9(4) . 1_455
O13 C2 O11 61.3(3) 5_566 1_455
O10 C2 O11 161.3(3) . 1_455
O10 C2 O11 23.6(3) 1_455 1_455
N2 C2 O11 76.2(2) . .
C2 C2 O11 87.9(4) 6_556 .
O13 C2 O11 61.3(3) . .
O13 C2 O11 150.9(4) 5_566 .
O10 C2 O11 23.6(3) . .
O10 C2 O11 161.3(3) 1_455 .
O11 C2 O11 144.39(13) 1_455 .
N2 C2 O11 85.7(2) . 5_656
C2 C2 O11 71.4(3) 6_556 5_656
O13 C2 O11 59.2(3) . 5_656
O13 C2 O11 140.5(4) 5_566 5_656
O10 C2 O11 22.6(3) . 5_656
O10 C2 O11 147.5(3) 1_455 5_656
O11 C2 O11 139.52(10) 1_455 5_656
O11 C2 O11 16.6(7) . 5_656
N2 C2 O11 85.7(2) . 5_556
C2 C2 O11 71.4(3) 6_556 5_556
O13 C2 O11 140.5(4) . 5_556
O13 C2 O11 59.2(3) 5_566 5_556
O10 C2 O11 147.5(3) . 5_556
O10 C2 O11 22.6(3) 1_455 5_556
O11 C2 O11 16.6(7) 1_455 5_556
O11 C2 O11 139.52(10) . 5_556
O11 C2 O11 129.1(5) 5_656 5_556
N2 C2 O12 117.1(4) . .
C2 C2 O12 80.00(5) 6_556 .
O13 C2 O12 17.4(5) . .
O13 C2 O12 107.8(5) 5_566 .
O10 C2 O12 21.1(5) . .
O10 C2 O12 143.4(4) 1_455 .
O11 C2 O12 165.5(4) 1_455 .
O11 C2 O12 43.9(4) . .
O11 C2 O12 42.9(4) 5_656 .
O11 C2 O12 150.3(4) 5_556 .
N2 C2 O12 117.1(4) . 1_455
C2 C2 O12 80.00(5) 6_556 1_455
O13 C2 O12 107.8(5) . 1_455
O13 C2 O12 17.4(5) 5_566 1_455
O10 C2 O12 143.4(4) . 1_455
O10 C2 O12 21.1(5) 1_455 1_455
O11 C2 O12 43.9(4) 1_455 1_455
O11 C2 O12 165.5(4) . 1_455
O11 C2 O12 150.3(4) 5_656 1_455
O11 C2 O12 42.9(4) 5_556 1_455
O12 C2 O12 124.9(8) . 1_455
N2 C2 H2 119.0 . .
C2 C2 H2 119.0 6_556 .
O13 C2 H2 60.6 . .
O13 C2 H2 60.6 5_566 .
O10 C2 H2 91.6 . .
O10 C2 H2 91.6 1_455 .
O11 C2 H2 106.4 1_455 .
O11 C2 H2 106.4 . .
O11 C2 H2 114.0 5_656 .
O11 C2 H2 114.0 5_556 .
O12 C2 H2 73.1 . .
O12 C2 H2 73.1 1_455 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ni1 C1 1.866(3) 5_665
Ni1 C1 1.866(3) .
Ni1 C1 1.866(3) 3_565
Ni1 C1 1.866(3) 7_655
Ni1 O12 3.443(6) 5_666
Ni1 O12 3.443(6) 1_554
Ni1 O12 3.443(6) .
Ni1 O12 3.443(6) 5_665
Ni1 O13 3.566(8) 5_666
Ni1 O13 3.566(8) 1_554
Ni1 O13 3.566(8) .
Ni1 O13 3.566(8) 5_665
Fe1 N1 1.944(3) .
Fe1 N1 1.944(3) 5
Fe1 N1 1.944(3) 3
Fe1 N1 1.944(3) 7
Fe1 N2 1.986(3) 5
Fe1 N2 1.986(3) .
Fe1 O11 4.544(15) 5
Fe1 O11 4.544(15) .
Fe1 O11 4.544(15) 5_655
Fe1 O11 4.544(15) 1_455
O10 O12 1.45(4) .
O10 O11 1.511(17) .
O10 O11 1.511(17) 5_656
O10 O13 2.332(18) 5_666
O10 O13 2.332(18) .
O10 O12 2.65(4) 5_666
O10 O10 2.81(3) 5_656
O10 C2 3.6345(13) .
O10 C2 3.6345(13) 6_656
O10 C2 3.6345(13) 6_556
O10 C2 3.6345(13) 1_655
O10 C1 3.719(3) 7_656
O10 C1 3.719(3) .
O10 C1 3.719(3) 1_556
O10 C1 3.719(3) 7_655
O10 Ni1 3.963(8) 1_556
O10 N1 4.0260(13) 7_656
O10 N1 4.0260(13) .
O10 N1 4.0260(13) 7_655
O11 O11 1.12(5) 5_656
O11 O10 1.511(17) 5_656
O11 O12 2.91(3) .
O11 O12 2.91(3) 5_656
O11 N2 3.655(6) .
O11 N2 3.655(6) 1_655
O11 O13 3.672(9) 5_666
O11 O13 3.672(9) 1_545
O11 O13 3.672(9) .
O11 O13 3.672(9) 5_656
O11 C2 3.7358(13) 2
O11 C2 3.7358(13) 1_655
O11 C2 3.7358(13) 2_655
O11 C2 3.7358(13) .
O11 C1 3.795(19) 3
O11 C1 3.795(19) 5_655
O11 C1 3.795(19) .
O11 C1 3.795(19) 7_655
O11 N1 3.817(19) 3
O12 O12 1.20(7) 5_666
O12 O13 1.26(3) 5_666
O12 O13 1.26(3) .
O12 O10 2.65(4) 5_666
O12 O11 2.91(3) 5_656
O12 Ni1 3.443(6) 1_556
O12 C1 3.710(7) .
O12 C1 3.710(7) 7_656
O12 C1 3.710(7) 7_655
O12 C1 3.710(7) 1_556
O12 C2 4.012(15) .
O12 C2 4.012(15) 6_556
O12 C2 4.012(15) 6_656
O12 C2 4.012(15) 1_655
O12 O11 4.10(3) 5_666
O12 O11 4.10(3) 1_565
O12 C1 4.112(16) 5_666
O13 O12 1.26(3) 5_666
O13 O13 2.21(5) 5_666
O13 O10 2.332(18) 5_666
O13 C2 3.446(18) .
O13 C2 3.446(18) 6_556
O13 C2 3.446(18) 5_566
O13 C2 3.446(18) 2_565
O13 Ni1 3.566(8) 1_556
O13 C1 3.6396(19) .
O13 C1 3.6396(19) 3_566
O13 C1 3.6396(19) 3_565
O13 C1 3.6396(19) 1_556
O13 O11 3.672(9) 5_666
O13 O11 3.672(9) 1_565
O13 O11 3.672(9) 5_656
O13 N1 4.123(7) .
N1 C1 1.149(4) .
N1 O11 3.817(19) 5_655
N1 O10 4.0260(13) 1_554
N1 O13 4.123(7) 1_554
N2 C2 1.337(3) .
N2 C2 1.337(3) 2
N2 O11 3.655(6) 1_455
N2 O11 4.064(12) 5_656
N2 O11 4.064(12) 5_556
N2 O10 4.073(6) 5_556
N2 O10 4.073(6) 5_656
N2 O10 4.073(6) 1_455
C1 O13 3.6396(19) 1_554
C1 O12 3.710(7) 1_554
C1 O10 3.719(3) 1_554
C1 O11 3.795(19) 5_655
C1 O12 4.112(16) 5_666
C1 O12 4.112(16) 5_665
C2 C2 1.394(6) 6_556
C2 O13 3.446(18) 5_566
C2 O10 3.6345(13) 1_455
C2 O11 3.7358(14) 1_455
C2 O11 3.940(8) 5_656
C2 O11 3.940(8) 5_556
C2 O12 4.012(15) 1_455
C2 H2 0.9500 .
